Improving waterborne coatings using a formulated nanoparticle
Improving waterborne coatings using a
formulated nanoparticle additive Oxylink
S. Pilotek* K. Steingroever** and M. Herold**
* Buhler Inc.
Business Unit Nanotechnology, Austin, TX 78701
**Buhler PARTEC GmbH
Saarbrücken, Germany 66123
Presented at the 15th International Coating Science and Technology Symposium,
September 13-15, 2010, St. Paul, MN1
Waterborne coatings have several important benefits over solvent borne alternatives. Stricter
regulations worldwide to lower VOC emissions are the main reason for a use of waterborne
solutions. However, in addition, waterborne coatings have the benefit of being less hazardous in
the application, as they do not emit hazardous fumes and odors, not flammable, and safe clean up
We present a study on the nanoparticle additive Oxylink™ that increases the crosslink
density of waterborne coatings. Previous studies have focused on the use of nanoparticles to
increase mechanical properties such as scratch resistance as well as UV protection by mineral
Generally, the key to functional nanoparticle coating additives comprises particles in a
stable dispersion that is compatible in the application. The intended interaction between polymer
and particle surface requires that the surface has sufficient accessibility for the polymer. The
degree of dispersion of the particle system has therefore a strong influence on the efficacy of the
resulting additive. We have previously discussed the topic of processing nanopowders into
functional colloids in more detail2. Dispersing nanopowders into functional colloids requires a
deagglomeration step. We have found the use of agitator bead mills useful for this part when the
particle surface is chemically stabilized at the same time. This concurrent action of mechanical
and chemical forces on agglomerated particles is called chemomechanical processing. We have
used this process to disperse a ZnO nanopowder in water and to formulate it as a coating
Unpublished. ISCST shall not be responsible for statements or opinions contained in papers or
printed in its publications.
See e.g., S. Pilotek, S. Schär, K. Steingröver, K. Gossmann, F. Tabellion, NSTI-Nanotech 2007,
Vol. 2, 64 (2007). S. Pilotek, D. Burgard, M. Herold, K. Steingröver, The Waterborne
Symposium 2009, New Orleans, LA (2009).
additive. The dispersion has a low viscosity of < 10 mPa·s at a solid content of ca. 40 wt.-%.
The dispersion has a pH value of 8. The material under investigation in this study is
commercially available in three versions under the trade name Oxylink™. The three types allow
to cover a broader range of formulations. For this study, the most suitable type of Oxylink™ was
Table 1 a, b shows the formulations W1 and M1 used in this study for wood and metal,
Table 1: Formulations discussed in this study
a) Exterior translucent high build stain (HBST) for
wood based on Primal AC 337 “W1”
b) Direct-to-metal coating based on Neocryl XK-86
PRIMAL™ AC337 ER (45.5%)
TEGO® Foamex 825
Aqueous ammonia (28%)
Nanoparticles Oxylink™ 3103
Acrysol™ RM12W (19%)
Surfynol 104 (50 %. in Etylene glycol)
Ti Pure R706
Mix ingredients in the given order and grind
Premix 2 (mix separately)
Adjust pH to 8.5 with aq. ammonia (15 %)
Premix 3 (mix separately)
Erbslöh flash rust inhibitor
CHE Coat LNF A4
Mix well, adjust pH to 8.5 with aq. ammonia (conc.) and
add while stirring to Premix 2. Homogenize for 5 min.
0.0 / 0.8
Add the resulting mixture to the Pigment Grind D 1855-4
while stirring, homogenize with rotor stator device, then
add while stirring:
0.0 / 0.8
Nanoparticles Oxylink™ 3101
Homogenize well for additional 5 min.
We have used the solvent-rub resistance test according to ASTM 5402 as a benchmark to
characterize the effect of Oxylink on latex coatings. In this test, a solvent-soaked cloth (methyl
ethyl ketone, MEK) is used to remove a coating from a glass substrate. A higher number of
double rubs characterizes a higher cross link density in the film. We have used the same test also
using iso-propanol (IPA). We find that the nanoparticle additive consistently increases the
number of MEK-double rubs by a factor of 4-6. Likewise, the number of IPA-double rubs is
increased by 30 – 50%, see figure 1. We attribute the different response to the different swelling
behavior of the latices with MEK and IPA, respectively, where the latter is more polar and protic
in contrast to the ketone. We propose that the difference in is an indication for the non-covalent
nature of the cross linking by the inorganic particles.
Figure 1: Solvent-rub test for formulations M1 and W1 with MEK and IPA
without (left bars, horizontal stripes) and with (right bars, diagonal stripes) Oxylink.
As a consequence of the increased cross link density further coating properties are
significantly improved. E.g., metal coating M1 as well as other metal formulations gains
improved humidity and weathering resistance with Oxylink as compared to the same
formulations without the additive (figure 2). The degree of blistering is markedly reduced.
Figure 2: Humidity resistance of formulation M1 and another metal formulation M2 without (left bars,
horizontal stripes) and with (right bars, diagonal stripes) Oxylink.
0: No blisters, 5: Complete failure due to blistering.
For the wood coating formulation W1 we evaluated the drying time and blocking
resistance as properties of special interest. Both parameters are positively and significantly
affected. The rate of blocking resistance is improved from 5 (complete blocking) to 1 under
increased temperature conditions on both Leneta™ foil and standardized fir plates (figure 3).
Interestingly, also the time to through-dry was reduced by half. We attribute this effect to a fast
kinetics of the Oxylink-resin interaction so that a certain grade of drying is reached after a
shorter period of time. Consequently, Oxylink results in improved values for resistances in early
water and chemical impact.
Figure 3L Blocking Resistance of W1 and another wood formulation W2 on Leneta foil without (left bars,
horizontally striped) and with (right bars, dotted) Oxylink.
Left set: Increased humidity conditions. Right set: Increased temperature conditions.
0: no blocking, 5: complete failure due to blocking.
In summary, we present a formulated performance additive based on ZnO nanoparticle
dispersions. The additive improves the general property profile of waterborne coatings by
increasing the cross- link density of the systems. The coatings benefit from higher resistance
properties against, e.g., humidity, solvent rubs, and blocking as well as from a decreased time to